The crystal structure described by Li4Ti3Ni3(WO8)2 is Hausmannite-derived structured and crystallizes in the triclinic P1 space group. There are four inequivalent Li sites. In the first Li site, Li(1) is bonded to one O(11), one O(12), one O(15), and one O(3) atom to form LiO4 tetrahedra that share  a cornercorner with one Ti(1)O6 octahedra,  a cornercorner with one Ti(2)O6 octahedra,  a cornercorner with one Ni(1)O6 octahedra, corners with two equivalent Ti(3)O6 octahedra, corners with two equivalent Ni(2)O6 octahedra, corners with two equivalent Ni(3)O6 octahedra, and corners with three equivalent W(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 51-65°. In the second Li site, Li(2) is bonded in a rectangular see-saw-like geometry to one O(14), one O(16), one O(5), and one O(9) atom. In the third Li site, Li(3) is bonded to one O(1), one O(10), one O(4), and one O(6) atom to form LiO4 tetrahedra that share  a cornercorner with one Ti(1)O6 octahedra,  a cornercorner with one Ti(2)O6 octahedra,  a cornercorner with one Ni(1)O6 octahedra, corners with three equivalent W(1)O6 octahedra,  an edgeedge with one Ti(3)O6 octahedra,  an edgeedge with one Ni(2)O6 octahedra, and  an edgeedge with one Ni(3)O6 octahedra. The corner-sharing octahedral tilt angles range from 54-64°. In the fourth Li site, Li(4) is bonded to one O(13), one O(2), one O(7), and one O(8) atom to form LiO4 tetrahedra that share  a cornercorner with one Ti(3)O6 octahedra,  a cornercorner with one Ni(2)O6 octahedra,  a cornercorner with one Ni(3)O6 octahedra, corners with two equivalent Ti(1)O6 octahedra, corners with two equivalent Ti(2)O6 octahedra, corners with two equivalent Ni(1)O6 octahedra, and corners with three equivalent W(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 51-65°. There are three inequivalent Ti sites. In the first Ti site, Ti(1) is bonded to one O(14), one O(2), one O(3), one O(4), one O(7), and one O(9) atom to form TiO6 octahedra that share corners with two equivalent W(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra,  a cornercorner with one Li(3)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  an edgeedge with one W(1)O6 octahedra, edges with two equivalent Ti(2)O6 octahedra, and edges with two equivalent Ni(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 48-51°. In the second Ti site, Ti(2) is bonded to one O(16), one O(2), one O(3), one O(4), one O(8), and one O(9) atom to form TiO6 octahedra that share corners with two equivalent W(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra,  a cornercorner with one Li(3)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  an edgeedge with one W(1)O6 octahedra, edges with two equivalent Ti(1)O6 octahedra, and edges with two equivalent Ni(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 49-51°. In the third Ti site, Ti(3) is bonded to one O(1), one O(11), one O(12), one O(13), one O(5), and one O(6) atom to form TiO6 octahedra that share corners with two equivalent W(1)O6 octahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one W(2)O6 octahedra, edges with two equivalent Ni(2)O6 octahedra, edges with two equivalent Ni(3)O6 octahedra, and  an edgeedge with one Li(3)O4 tetrahedra. The corner-sharing octahedral tilt angles range from 49-51°. There are two inequivalent W sites. In the first W site, W(1) is bonded to one O(1), one O(10), one O(2), one O(6), one O(7), and one O(8) atom to form WO6 octahedra that share corners with two equivalent Ti(3)O6 octahedra, corners with two equivalent Ni(2)O6 octahedra, corners with two equivalent Ni(3)O6 octahedra, corners with three equivalent Li(3)O4 tetrahedra, corners with three equivalent Li(4)O4 tetrahedra,  an edgeedge with one Ti(1)O6 octahedra,  an edgeedge with one Ti(2)O6 octahedra, and  an edgeedge with one Ni(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 49-52°. In the second W site, W(2) is bonded to one O(11), one O(12), one O(14), one O(15), one O(16), and one O(9) atom to form WO6 octahedra that share corners with two equivalent Ti(1)O6 octahedra, corners with two equivalent Ti(2)O6 octahedra, corners with two equivalent Ni(1)O6 octahedra, corners with three equivalent Li(1)O4 tetrahedra,  an edgeedge with one Ti(3)O6 octahedra,  an edgeedge with one Ni(2)O6 octahedra, and  an edgeedge with one Ni(3)O6 octahedra. The corner-sharing octahedral tilt angles range from 48-52°. There are three inequivalent Ni sites. In the first Ni site, Ni(1) is bonded to one O(14), one O(16), one O(3), one O(4), one O(7), and one O(8) atom to form NiO6 octahedra that share corners with two equivalent W(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra,  a cornercorner with one Li(3)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  an edgeedge with one W(1)O6 octahedra, edges with two equivalent Ti(1)O6 octahedra, and edges with two equivalent Ti(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 51-52°. In the second Ni site, Ni(2) is bonded to one O(1), one O(10), one O(11), one O(13), one O(15), and one O(5) atom to form NiO6 octahedra that share corners with two equivalent W(1)O6 octahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one W(2)O6 octahedra, edges with two equivalent Ti(3)O6 octahedra, edges with two equivalent Ni(3)O6 octahedra, and  an edgeedge with one Li(3)O4 tetrahedra. The corner-sharing octahedral tilt angles are 50°. In the third Ni site, Ni(3) is bonded to one O(10), one O(12), one O(13), one O(15), one O(5), and one O(6) atom to form NiO6 octahedra that share corners with two equivalent W(1)O6 octahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one W(2)O6 octahedra, edges with two equivalent Ti(3)O6 octahedra, edges with two equivalent Ni(2)O6 octahedra, and  an edgeedge with one Li(3)O4 tetrahedra. The corner-sharing octahedral tilt angles are 52°. There are sixteen inequivalent O sites. In the first O site, O(1) is bonded in a rectangular see-saw-like geometry to one Li(3), one Ti(3), one W(1), and one Ni(2) atom. In the second O site, O(2) is bonded to one Li(4), one Ti(1), one Ti(2), and one W(1) atom to form distorted OLiTi2W tetrahedra that share  a cornercorner with one O(7)LiTiNiW tetrahedra,  a cornercorner with one O(8)LiTiNiW tetrahedra, corners with two equivalent O(4)LiTi2Ni tetrahedra,  an edgeedge with one O(7)LiTiNiW tetrahedra, and  an edgeedge with one O(8)LiTiNiW tetrahedra. In the third O site, O(3) is bonded in a distorted rectangular see-saw-like geometry to one Li(1), one Ti(1), one Ti(2), and one Ni(1) atom. In the fourth O site, O(4) is bonded to one Li(3), one Ti(1), one Ti(2), and one Ni(1) atom to form OLiTi2Ni tetrahedra that share corners with two equivalent O(2)LiTi2W tetrahedra, corners with two equivalent O(7)LiTiNiW tetrahedra, and corners with two equivalent O(8)LiTiNiW tetrahedra. In the fifth O site, O(5) is bonded to one Li(2), one Ti(3), one Ni(2), and one Ni(3) atom to form corner-sharing OLiTiNi2 tetrahedra. In the sixth O site, O(6) is bonded in a rectangular see-saw-like geometry to one Li(3), one Ti(3), one W(1), and one Ni(3) atom. In the seventh O site, O(7) is bonded to one Li(4), one Ti(1), one W(1), and one Ni(1) atom to form distorted OLiTiNiW tetrahedra that share  a cornercorner with one O(2)LiTi2W tetrahedra,  a cornercorner with one O(8)LiTiNiW tetrahedra, corners with two equivalent O(4)LiTi2Ni tetrahedra,  an edgeedge with one O(2)LiTi2W tetrahedra, and  an edgeedge with one O(8)LiTiNiW tetrahedra. In the eighth O site, O(8) is bonded to one Li(4), one Ti(2), one W(1), and one Ni(1) atom to form distorted OLiTiNiW tetrahedra that share  a cornercorner with one O(2)LiTi2W tetrahedra,  a cornercorner with one O(7)LiTiNiW tetrahedra, corners with two equivalent O(4)LiTi2Ni tetrahedra,  an edgeedge with one O(2)LiTi2W tetrahedra, and  an edgeedge with one O(7)LiTiNiW tetrahedra. In the ninth O site, O(9) is bonded in a rectangular see-saw-like geometry to one Li(2), one Ti(1), one Ti(2), and one W(2) atom. In the tenth O site, O(10) is bonded in a rectangular see-saw-like geometry to one Li(3), one W(1), one Ni(2), and one Ni(3) atom. In the eleventh O site, O(11) is bonded in a rectangular see-saw-like geometry to one Li(1), one Ti(3), one W(2), and one Ni(2) atom. In the twelfth O site, O(12) is bonded in a distorted rectangular see-saw-like geometry to one Li(1), one Ti(3), one W(2), and one Ni(3) atom. In the thirteenth O site, O(13) is bonded in a rectangular see-saw-like geometry to one Li(4), one Ti(3), one Ni(2), and one Ni(3) atom. In the fourteenth O site, O(14) is bonded in a rectangular see-saw-like geometry to one Li(2), one Ti(1), one W(2), and one Ni(1) atom. In the fifteenth O site, O(15) is bonded to one Li(1), one W(2), one Ni(2), and one Ni(3) atom to form distorted corner-sharing OLiNi2W tetrahedra. In the sixteenth O site, O(16) is bonded in a rectangular see-saw-like geometry to one Li(2), one Ti(2), one W(2), and one Ni(1) atom. is represented by the CIF card [CIF]
data_Li4Ti3Ni3(WO8)2
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   5.991
_cell_length_b   5.949
_cell_length_c   9.749
_cell_angle_alpha   90.286
_cell_angle_beta   90.898
_cell_angle_gamma   120.019
_symmetry_Int_Tables_number   1
_cell_volume   300.760
_cell_formula_units_Z   1
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Li  Li0  1  0.324  0.661  0.900  1.0
  Li  Li1  1  0.988  0.994  0.984  1.0
  Li  Li2  1  0.004  0.001  0.496  1.0
  Li  Li3  1  0.666  0.335  0.409  1.0
  Ti  Ti4  1  0.184  0.843  0.217  1.0
  Ti  Ti5  1  0.175  0.339  0.214  1.0
  Ti  Ti6  1  0.343  0.180  0.719  1.0
  Ni  Ni7  1  0.660  0.831  0.209  1.0
  Ni  Ni8  1  0.838  0.659  0.710  1.0
  Ni  Ni9  1  0.836  0.176  0.710  1.0
  W  W10  1  0.344  0.673  0.491  1.0
  W  W11  1  0.682  0.341  0.982  1.0
  O  O12  1  0.173  0.834  0.593  1.0
  O  O13  1  0.042  0.521  0.340  1.0
  O  O14  1  0.311  0.656  0.107  1.0
  O  O15  1  0.008  0.001  0.306  1.0
  O  O16  1  0.012  0.008  0.799  1.0
  O  O17  1  0.181  0.340  0.596  1.0
  O  O18  1  0.467  0.967  0.342  1.0
  O  O19  1  0.467  0.506  0.339  1.0
  O  O20  1  0.331  0.164  0.105  1.0
  O  O21  1  0.663  0.830  0.583  1.0
  O  O22  1  0.507  0.475  0.848  1.0
  O  O23  1  0.500  0.037  0.857  1.0
  O  O24  1  0.641  0.314  0.608  1.0
  O  O25  1  0.840  0.659  0.095  1.0
  O  O26  1  0.963  0.482  0.850  1.0
  O  O27  1  0.847  0.175  0.097  1.0
[/CIF]
.
The crystal structure described by Li4Ti3Ni3(WO8)2 is Hausmannite-derived structured and crystallizes in the triclinic P1 space group. There are four inequivalent Li sites. In the first Li site, Li(1) is bonded to one O(11), one O(12), one O(15), and one O(3) atom to form LiO4 tetrahedra that share  a cornercorner with one Ti(1)O6 octahedra,  a cornercorner with one Ti(2)O6 octahedra,  a cornercorner with one Ni(1)O6 octahedra, corners with two equivalent Ti(3)O6 octahedra, corners with two equivalent Ni(2)O6 octahedra, corners with two equivalent Ni(3)O6 octahedra, and corners with three equivalent W(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 51-65°. In the second Li site, Li(2) is bonded in a rectangular see-saw-like geometry to one O(14), one O(16), one O(5), and one O(9) atom. In the third Li site, Li(3) is bonded to one O(1), one O(10), one O(4), and one O(6) atom to form LiO4 tetrahedra that share  a cornercorner with one Ti(1)O6 octahedra,  a cornercorner with one Ti(2)O6 octahedra,  a cornercorner with one Ni(1)O6 octahedra, corners with three equivalent W(1)O6 octahedra,  an edgeedge with one Ti(3)O6 octahedra,  an edgeedge with one Ni(2)O6 octahedra, and  an edgeedge with one Ni(3)O6 octahedra. The corner-sharing octahedral tilt angles range from 54-64°. In the fourth Li site, Li(4) is bonded to one O(13), one O(2), one O(7), and one O(8) atom to form LiO4 tetrahedra that share  a cornercorner with one Ti(3)O6 octahedra,  a cornercorner with one Ni(2)O6 octahedra,  a cornercorner with one Ni(3)O6 octahedra, corners with two equivalent Ti(1)O6 octahedra, corners with two equivalent Ti(2)O6 octahedra, corners with two equivalent Ni(1)O6 octahedra, and corners with three equivalent W(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 51-65°. There are three inequivalent Ti sites. In the first Ti site, Ti(1) is bonded to one O(14), one O(2), one O(3), one O(4), one O(7), and one O(9) atom to form TiO6 octahedra that share corners with two equivalent W(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra,  a cornercorner with one Li(3)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  an edgeedge with one W(1)O6 octahedra, edges with two equivalent Ti(2)O6 octahedra, and edges with two equivalent Ni(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 48-51°. In the second Ti site, Ti(2) is bonded to one O(16), one O(2), one O(3), one O(4), one O(8), and one O(9) atom to form TiO6 octahedra that share corners with two equivalent W(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra,  a cornercorner with one Li(3)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  an edgeedge with one W(1)O6 octahedra, edges with two equivalent Ti(1)O6 octahedra, and edges with two equivalent Ni(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 49-51°. In the third Ti site, Ti(3) is bonded to one O(1), one O(11), one O(12), one O(13), one O(5), and one O(6) atom to form TiO6 octahedra that share corners with two equivalent W(1)O6 octahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one W(2)O6 octahedra, edges with two equivalent Ni(2)O6 octahedra, edges with two equivalent Ni(3)O6 octahedra, and  an edgeedge with one Li(3)O4 tetrahedra. The corner-sharing octahedral tilt angles range from 49-51°. There are two inequivalent W sites. In the first W site, W(1) is bonded to one O(1), one O(10), one O(2), one O(6), one O(7), and one O(8) atom to form WO6 octahedra that share corners with two equivalent Ti(3)O6 octahedra, corners with two equivalent Ni(2)O6 octahedra, corners with two equivalent Ni(3)O6 octahedra, corners with three equivalent Li(3)O4 tetrahedra, corners with three equivalent Li(4)O4 tetrahedra,  an edgeedge with one Ti(1)O6 octahedra,  an edgeedge with one Ti(2)O6 octahedra, and  an edgeedge with one Ni(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 49-52°. In the second W site, W(2) is bonded to one O(11), one O(12), one O(14), one O(15), one O(16), and one O(9) atom to form WO6 octahedra that share corners with two equivalent Ti(1)O6 octahedra, corners with two equivalent Ti(2)O6 octahedra, corners with two equivalent Ni(1)O6 octahedra, corners with three equivalent Li(1)O4 tetrahedra,  an edgeedge with one Ti(3)O6 octahedra,  an edgeedge with one Ni(2)O6 octahedra, and  an edgeedge with one Ni(3)O6 octahedra. The corner-sharing octahedral tilt angles range from 48-52°. There are three inequivalent Ni sites. In the first Ni site, Ni(1) is bonded to one O(14), one O(16), one O(3), one O(4), one O(7), and one O(8) atom to form NiO6 octahedra that share corners with two equivalent W(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra,  a cornercorner with one Li(3)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  an edgeedge with one W(1)O6 octahedra, edges with two equivalent Ti(1)O6 octahedra, and edges with two equivalent Ti(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 51-52°. In the second Ni site, Ni(2) is bonded to one O(1), one O(10), one O(11), one O(13), one O(15), and one O(5) atom to form NiO6 octahedra that share corners with two equivalent W(1)O6 octahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one W(2)O6 octahedra, edges with two equivalent Ti(3)O6 octahedra, edges with two equivalent Ni(3)O6 octahedra, and  an edgeedge with one Li(3)O4 tetrahedra. The corner-sharing octahedral tilt angles are 50°. In the third Ni site, Ni(3) is bonded to one O(10), one O(12), one O(13), one O(15), one O(5), and one O(6) atom to form NiO6 octahedra that share corners with two equivalent W(1)O6 octahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one W(2)O6 octahedra, edges with two equivalent Ti(3)O6 octahedra, edges with two equivalent Ni(2)O6 octahedra, and  an edgeedge with one Li(3)O4 tetrahedra. The corner-sharing octahedral tilt angles are 52°. There are sixteen inequivalent O sites. In the first O site, O(1) is bonded in a rectangular see-saw-like geometry to one Li(3), one Ti(3), one W(1), and one Ni(2) atom. In the second O site, O(2) is bonded to one Li(4), one Ti(1), one Ti(2), and one W(1) atom to form distorted OLiTi2W tetrahedra that share  a cornercorner with one O(7)LiTiNiW tetrahedra,  a cornercorner with one O(8)LiTiNiW tetrahedra, corners with two equivalent O(4)LiTi2Ni tetrahedra,  an edgeedge with one O(7)LiTiNiW tetrahedra, and  an edgeedge with one O(8)LiTiNiW tetrahedra. In the third O site, O(3) is bonded in a distorted rectangular see-saw-like geometry to one Li(1), one Ti(1), one Ti(2), and one Ni(1) atom. In the fourth O site, O(4) is bonded to one Li(3), one Ti(1), one Ti(2), and one Ni(1) atom to form OLiTi2Ni tetrahedra that share corners with two equivalent O(2)LiTi2W tetrahedra, corners with two equivalent O(7)LiTiNiW tetrahedra, and corners with two equivalent O(8)LiTiNiW tetrahedra. In the fifth O site, O(5) is bonded to one Li(2), one Ti(3), one Ni(2), and one Ni(3) atom to form corner-sharing OLiTiNi2 tetrahedra. In the sixth O site, O(6) is bonded in a rectangular see-saw-like geometry to one Li(3), one Ti(3), one W(1), and one Ni(3) atom. In the seventh O site, O(7) is bonded to one Li(4), one Ti(1), one W(1), and one Ni(1) atom to form distorted OLiTiNiW tetrahedra that share  a cornercorner with one O(2)LiTi2W tetrahedra,  a cornercorner with one O(8)LiTiNiW tetrahedra, corners with two equivalent O(4)LiTi2Ni tetrahedra,  an edgeedge with one O(2)LiTi2W tetrahedra, and  an edgeedge with one O(8)LiTiNiW tetrahedra. In the eighth O site, O(8) is bonded to one Li(4), one Ti(2), one W(1), and one Ni(1) atom to form distorted OLiTiNiW tetrahedra that share  a cornercorner with one O(2)LiTi2W tetrahedra,  a cornercorner with one O(7)LiTiNiW tetrahedra, corners with two equivalent O(4)LiTi2Ni tetrahedra,  an edgeedge with one O(2)LiTi2W tetrahedra, and  an edgeedge with one O(7)LiTiNiW tetrahedra. In the ninth O site, O(9) is bonded in a rectangular see-saw-like geometry to one Li(2), one Ti(1), one Ti(2), and one W(2) atom. In the tenth O site, O(10) is bonded in a rectangular see-saw-like geometry to one Li(3), one W(1), one Ni(2), and one Ni(3) atom. In the eleventh O site, O(11) is bonded in a rectangular see-saw-like geometry to one Li(1), one Ti(3), one W(2), and one Ni(2) atom. In the twelfth O site, O(12) is bonded in a distorted rectangular see-saw-like geometry to one Li(1), one Ti(3), one W(2), and one Ni(3) atom. In the thirteenth O site, O(13) is bonded in a rectangular see-saw-like geometry to one Li(4), one Ti(3), one Ni(2), and one Ni(3) atom. In the fourteenth O site, O(14) is bonded in a rectangular see-saw-like geometry to one Li(2), one Ti(1), one W(2), and one Ni(1) atom. In the fifteenth O site, O(15) is bonded to one Li(1), one W(2), one Ni(2), and one Ni(3) atom to form distorted corner-sharing OLiNi2W tetrahedra. In the sixteenth O site, O(16) is bonded in a rectangular see-saw-like geometry to one Li(2), one Ti(2), one W(2), and one Ni(1) atom. is represented by the CIF card [CIF]
data_Li4Ti3Ni3(WO8)2
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   5.991
_cell_length_b   5.949
_cell_length_c   9.749
_cell_angle_alpha   90.286
_cell_angle_beta   90.898
_cell_angle_gamma   120.019
_symmetry_Int_Tables_number   1
_cell_volume   300.760
_cell_formula_units_Z   1
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Li  Li0  1  0.324  0.661  0.900  1.0
  Li  Li1  1  0.988  0.994  0.984  1.0
  Li  Li2  1  0.004  0.001  0.496  1.0
  Li  Li3  1  0.666  0.335  0.409  1.0
  Ti  Ti4  1  0.184  0.843  0.217  1.0
  Ti  Ti5  1  0.175  0.339  0.214  1.0
  Ti  Ti6  1  0.343  0.180  0.719  1.0
  Ni  Ni7  1  0.660  0.831  0.209  1.0
  Ni  Ni8  1  0.838  0.659  0.710  1.0
  Ni  Ni9  1  0.836  0.176  0.710  1.0
  W  W10  1  0.344  0.673  0.491  1.0
  W  W11  1  0.682  0.341  0.982  1.0
  O  O12  1  0.173  0.834  0.593  1.0
  O  O13  1  0.042  0.521  0.340  1.0
  O  O14  1  0.311  0.656  0.107  1.0
  O  O15  1  0.008  0.001  0.306  1.0
  O  O16  1  0.012  0.008  0.799  1.0
  O  O17  1  0.181  0.340  0.596  1.0
  O  O18  1  0.467  0.967  0.342  1.0
  O  O19  1  0.467  0.506  0.339  1.0
  O  O20  1  0.331  0.164  0.105  1.0
  O  O21  1  0.663  0.830  0.583  1.0
  O  O22  1  0.507  0.475  0.848  1.0
  O  O23  1  0.500  0.037  0.857  1.0
  O  O24  1  0.641  0.314  0.608  1.0
  O  O25  1  0.840  0.659  0.095  1.0
  O  O26  1  0.963  0.482  0.850  1.0
  O  O27  1  0.847  0.175  0.097  1.0
[/CIF]
.